85SBioglass, Sol-Gel, Polycaprolactone, Composites, <i>In
vitro</i> BioactivityInternational Journal of Materials and
Chemistry 2013, 3(5): 91-98 DOI: 10.5923/j.ijmc.20130305.02
In vitro Bioactivity of Polycaprolactone/Bioglass Composites
Lachezar Radev1,*, Dimitar Vladov1, Irena Michailova2, Ekaterina
Cholakova1, Maria F. V. Fernandes3, Isabel M. M. Salvado3
1Department of Fundamental Chemical Technology, University of
Chemical Technology and Metallurgy, Sofia, 1756, Bulgaria
2Department of Silicate Technology, University of Chemical
Technology and Metallurgy, Sofia, 1756, Bulgaria 3Materials
Engineering and Ceramics Department, CICECO, University of Aveiro,
3810-193 AVEIRO, Portugal
Abstract A series of Polycaprolactone and Bioglass in the
85SiO2-10CaO-5P2O5 (mol. %) systems were synthesized at different
quantity of the organic/inorganic components. The 85S Bioglass was
prepared via sol-gel method. It was added to the Polycaprolactone
matrix at 20, 50 and 80 weight (wt.) %, respectively. In vitro
bioactivity of the prepared composites was evaluated in 1.5
Simulated Body Flu id (1.5 SBF). The obtained composite materials
before and after static in vitro test were characterized by FTIR
and SEM. The obtained experimental data proved that the synthesized
composites exhibit good in vitro bioactivity. After immersion in
1.5SBF, SEM depicts the presence of nano-needle-like hydroxyapatite
on the immersed 20PCL/80BG and 50PCL/50BG samples.
Keywords 85SBioglass, Sol-Gel, Polycaprolactone, Composites, In
1. Introduction It is known that Polymer-Glass composites
enjoy the mechanical reliability of the polymer phase and the
excellent bioactiv ity of the g lassy phase. In this context
poly (-caprolactone) (PCL) is used to obtain different bioactive
composites, which are already referred in the recent publications,
focused on the production and application of PCL-based composites,
loaded with different inorganic phases, such as Bioglasses
(BG)[2-10], hydroxyapatite[7, 11-16], silica[17, 18], calcium
silicate, tri calcium phosphate (TCP)[7, 20], ZrO2,
TiO2, forsterite (Mg2SiO4) and hardystonite
(Ca2ZnSi2O7). On the other hand, the promot ion ro le of
silicon in bone metabolism was first observed by[25, 26]. Some
authors synthesized Si-substituted TCP and hydroxyapatite
(Si-HA) with different quantity of silicon. They observed
better bioactivity of these ceramics towards bone formation than
those without silicon.
In the field of PCL/BG composites some authors find that the
combinations of PCL/45S BG[2, 3] and PCL/Calcium Silicate BG
produce in vitro bioactivity, after soaking of the synthesized
composites in SBF for different t imes. The obtained new
precipitate promoted crystals with needle-like mo r p h o log y .
E. T a mij e t a l . [ 4 ] s tu d ied wh en
* Corresponding author: [email protected]
(Lachezar Radev) Published
online at http://journal.sapub.org/ijmc Copyright © 2013 Scientific
& Academic Publishing. All Rights Reserved
45SiO2-24.5Na2O-24.5CaO-6P2O5 (wt. %) BG was added to PCL, lower in
vitro b ioactivity acquired. M. Mohammadi et al., observed that
two types of BG, described as 50P2O5-40CaO-10SiO2 or 10Fe2O3 mixed
with PCL promote Brushite format ion after soaking in SBF solutions
for 14 and 28 days. H-H. Lee and colleagues synthesized in vitro
biodegradable composite in the presence of 70SiO2-25CaO-5P2O5 (mol.
%) nanofibrous BG and PCL. They concluded that the synthesized
composite membranes showed the rapid induction of apatite
precipitates on their surface. Furthermore, S. R oohani-Estefani
at al., prepared 58SiO2-38CaO-4P2O5 (mol. %) BG/PCL composites.
They demonstrated that the shape of the 58BG had significant
importance for bone regeneration. B. Lei et al., 
investigated that the addition of 60SiO2-36CaO-4P2O5 (mol. %) BG
enhanced in vitro bioactivity of the investigated composites.
Briefly, in spite of numerous publications on PCL/BG composites
information on the in vitro bioactivity of PCL/85S BG in 1.5 SBF
solutions does not exist.
In this study we have synthesized sol-gel glass in the
SiO2-CaO-P2O5 system with high silicon content (85 mol. %) and then
mixed it with PCL to prepare PCL/BG composites with different
content of PCL and BG. PCL was selected, because it has FDA
approval in several b iomimetic devises, low cost, and most of all,
it is slowly degradable. In vitro bioactivity of the prepared
PCL/BG composites were evaluated in 1.5 SBF solution.
2. Experimental Part
92 Lachezar Radev et al.: In vitro Bioactivity of
Preparation of BG and PCL/BG composites BG in the SiO2-CaO-P2O5
system was used as filler. BG
was synthesized via polystep sol-gel method. The composition was
described as 85SiO2-10CaO-5P2O5 (mol. %). The obtained BG was
denoted as 85S Bioglass. Tetraethoxysilane (TEOS) and phosphoric
acid (H3PO4) were used as sources. CaO was heated at 500 for 2
hours before using as Ca(OH)2 in water medium. The synthesis of 85S
Bioglass had already been described in.
Polycaprolactone (PCL) with Mw=6000 (Sigma-Aldrich) was dispersed
in 10 ml ch loroform then BG powder was added into PCL solution and
continuously stirred for 24 hours to disperse 85S BG uniformly.
After that the obtained mixture was heated at 50 under vacuum to
produce composites. The PCL/BG ratio were fixed as 50:50, 80:20 and
20:80 (wt. %). The synthesized composites were depicted as
50PCL/50BG, 80PCL/20BG and 20PCL/80 BG. Biomimetic surface
In the presented study, the treatments were conducted in 1.5 SBF
solution, to stimulate the nuclei formation on the composite
surface, in accordance by the method, described from Kokubo et.
The 1.5 SBF was prepared from d ifferent reagents as
follow: NaCl=11.925 g, NaHCO3=0.5295 g, KCl=0.3360 g, K2 HPO4
.3H2O=0.3420g, MgCl2 .6H2 O=0.4575g , CaCl2.2 H2O=0.5520g,
Na2SO4=0.106 g, and buffering at pH=7.4 at 36.5 with 9.0075 g of
TRIS and 1M HCl in distilled water. A few drops of NaN3 was added
to the 1.5 SBF to inhib it bacterial growth. After soaking, the
PCL/BG specimens were removed from the SBF solution, gently rinsed
with distilled water and then dried at 36.5 for 12 hours. Methods
FTIR spectroscopy was used to identify the functional groups of BG
powder and PCL/BG composites with different weight ratio of the
components. FTIR spectra were recordered using a Brucker Tensor 27
spectrometer equipped with MCT detector with a resolution of 4 cm-1
(64 scans). KBr pelletized discs containing 2 mg of sample and 200
mg KBr were made. SEM (Jeol, JSM-35CF, Japan) was used to ascertain
the morphology and chemical constituents of the prepared composites
before and after immersion in 1.5 SBF solution for 12 days at
accelerating voltage of 15 kv.
3. Results and Discussion
International Journal of Materials and Chemistry 2013, 3(5): 91-98
Figure 2. FTIR of pure PCL and PCL/BG composites at different
weight ratio of the components before in vitro test
Figure 3. Curve-fitt ing spectra of the 50PCL/50BG composite before
immersion in 1.5 SBF
4000 3500 3000 2500 2000 1500 1000 500 0
94 Lachezar Radev et al.: In vitro Bioactivity of
FTIR spectrum of the 85S BG after its stabilization at 700oC for 3
hours is given in Fig. 1.
Fig. 1 presents the spectrum of the 85S BG, which shows very strong
absorption peak at 1110 cm-1 assigned to Si-O-Si asymmetric
stretching mode and peaks centered at 797 and 465 cm-1 assigned
to the symmetric stretching and rocking v ibration of Si-O-Si band,
respectively[32, 33]. The peak at 3472 cm-1 could be ascribed to
the vibrat ion of different OH groups. The band with low
intensity at 565 cm-1corresponds to bending vibration of P-O bond
and suggests that the phosphate enters in 85S BG as network
former. Moreover, the absorption peak at 1632 cm-1 is
attributed to the water, absorbed on the surface Si-OH groups.
C. Vaid et al. concluded that the vibration bond, posited at ~1630
cm-1 and a broad band at 3000-3700 cm-1
was more p rominent in the case of g lasses, containing phosphorus
due to the presence of more surface Si-OH groups.
Typical spectra of PCL and PCL/BG composites are given in
The FTIR spectrum of pure PCL depicts the presence of carbonyl
(-C=O) stretching vibration at 1723 cm-1, labeled as ()[10-12, 23,
34]. Symmetric and asymmetric CH2 stretching mode at 2934 and 2864
cm-1 are also visible[3, 11, 24, 34, 35]. On the other hand, the
band at 1294 cm-1 could be ascribed to the backbone C-C and C-O
stretching vibrations in the crystalline phase of PCL[23, 24, 34,
35]. The band at ~1167 cm-1 which is assigned to the amorphous
phase of PCL[24, 35] is not visib le in our case. It is noteworthy
the presence of weak absorption peak at 1560 cm-1, attributable to
the antisymmetric stretching vibration of the COO- in 50PCL/50BG
and 80PCL/20BG composites . Furthermore, the band, centered
~700 cm-1 could be ascribed to the presence of Si-O-Si bond in the
sol-gel derived BG[32, 33]. B. Lei et al., proved that in the case
of Nanoscale Bioactive Glass (NBG), reinforced PCL composites, the
same band also been observed. The presence of this band can be
related to the presence of BG into the synthesized composites. As
can be seen from the presented in Figure 2 FTIR spectra, the
intensity of this band, labeled as (♦), is a function of weight
quantity of BG into the composites, i. e . this band is quite visib
le for the 20PCL/80BG composite (Fig. 2, curve 3).
The more detailed in formation about the presence of PCL and BG in
the 50PCL/50BG composite was analyzed by the curve-fitting in the
region 745-845 cm-1 (Fig. 3).
From the presented Fig. 3 it can be seen that the band, centered at
778 cm-1 could be ascribed to the PCL while the band at 803 cm-1
could be related to Si-O-Si in accordance with FTIR data, presented
in Fig. 1.
In addition, the well-defined, but not very intense, bands, posited
at ~570 cm-1 could be defined as P-O stretching modes of PO4
3- from 85S BG. The surface morphology of the prepared
composites before the in vitro test was studied by SEM as shown in
SEM image of the 50PCL/50BG (Fig. 4) shows that
85SBG has a good dispersion in the PCL matrix. On the other hand,
SEM shows the presence of large cavities, due to the removal of
chloroform which had previously been introduced during its
preparation. The sizes of these cavities are ~40 µm.
SEM of the 20PCL/80BG is given in Fig. 5
Fugure 4. SEMfor PCL50/50BG composite
Fugure 5. SEM for 20PCL/80BG
Fugure 6. SEM of 80PCL/20BG
From the presented SEM image it is visible that when the quantity
of BG increases, the quantity of particles attached on the PCL
surface also increase. From the depicted in Fig. 5 SEM image we
could also observe that the pore size decreased, compared with the
50PCL/50BG, presented in
International Journal of Materials and Chemistry 2013, 3(5): 91-98
Fig. 4. The SEM image also shows that the embedded BG particles
have different sizes from 2 to 15 µm. The cavities observed in the
sample have sizes s maller than those observed in the previous
sample (fig. 4). This is due to the quantity of the two components
from the prepared composite.
SEM of the composite with 80 wt.% PCL (80PCL/20BG) is presented in
Fig. 6 shows the morphology of the sample before exposure in 1.5
SBF solution. The SEM image illustrates that the surface of the
prepared composite is rough and porous. Almost no BG part icles
could be seen on the surface. In accordance with, this fact can
be related to the inclusion of BG part icles into the PCL
FTIR of the synthesized PCL/BG composites after in vitro test for 3
days are given in Fig. 7.
Figure 7. FTIR of the 50PCL/50BG, 20PCL/80BG and 80PLC/20BG
composites, after in vitro test in 1.5 SBF for 3 days in static
Figure 8. FTIR of the 50PCL/50BG, 20PCL/80BG and 80PLC/20BG
composites after in vitro test in 1.5 SBF for 12 days in static
4000 3500 3000 2500 2000 1500 1000 500
96 Lachezar Radev et al.: In vitro Bioactivity of
The FTIR spectra of the three PCL/BG composites with different
weight ratio of the PCL and BG after soaking in 1.5 SBF for 3 days,
showed that the intensities of the bands significantly decreased
with increasing of the immersion time up to 3 days of soaking,
compared with the FTIR spectra of PCL/BG before immersion (Fig. 2).
The decreasing of peaks intensity after the in vitro test was
attributed to the partial hydrolysis of the organic part of the
composites (PCL). This process is more visible for the –C=O bond,
presented from the absorption peak, posited at ~1720 cm-1, and
labeled as (). On the other hand, in 80PCL/20BG composite (Fig. 6,
curve 3), the intensity of the band at 797 cm-1 (labeled as ♦)
became more v isible. This peak could be ascribed to the Si-O-Si
vibrat ion mode of 85S BG (Fig. 1). This fact can be based also on
the process of partial dissolution of PCL in 1.5 SBF solution.
Furthermore, the P-O stretching modes of PO4
3- at ~570 cm-1 for the three composites are quite visible. These
peaks are indicative for calcium phosphate crystalline phases on
the surface of the soaked samples. Moreover, FTIR results presented
at Fig. 7 also depict the presence of CO3
2- bands at 1560, 1462 and 1400 cm-1 (for the 50PCL/50BG), 1530,
1460, 1392 and 1370 cm-1 (for 20PCL/80BG) and at 1436, 1420 and
1400 cm-1 (for 80PCL/20BG). The presence of these bands could be
related to the CO3HA formation on the surface o f the soaked
samples for 3 days in 1.5 SBF solution.
From the presented FTIR results we can summarize that: • After in
vitro test for 3 days, PCL partially dissolved
in to 1.5 SBF solution. • BG does not undergo any visible changes
immersion. • Some CO3
2- peaks could be observed for the three samples. On the base of
these conclusions we can conclude that the
synthesized PCL/BG composites are in vitro bioactive. The observed
results are in a good agreement with our preliminary studies
FTIR spectra of the prepared PCL/BG composites with different
weight ratio of the components after soaking in 1.5 SBF for 12 days
are given in Fig. 8.
After comparison of the presented at Fig. 7 FTIR spectra with those
depicted in Fig. 6 it is quite visible that after 12 days of
soaking, the intensity of the characteristic bonds increased. Based
on the obtained results, we can conclude that the synthesized
composites are covered with a new phase of crystalline calcium
phosphates. In this context, the peaks in the 1350-1550 cm-1 region
are associated with CO3
2- moieties (bending ν3 and ν4 modes). Moreover, the peaks
centered at 875 cm-1 (labeled as ) and those at 1415 (1421) cm-1,
1460 (1459) cm-1 could be ascribed to the presence of CO3
2- into HA lattice, i.e. on the surface CO3HA were formed[14-16].
Furthermore, peaks between 1000-1100 cm-1 are due to the triply
generated asymmetric stretching mode of P-O bonds in PO4
3-[5, 15, 16, 36, 37]. The peak, posited at 960 cm-1 could be
ascribed to HPO4
2-, incorporated into the lattice. This peak could be ascribed to
the dicalcium phosphate dihydrate (DCPD or Brushite) on the
surface after 12 days of immersion. Based on the presented FTIR
results we can conclude that
on the surface of the prepared PCL/BG composites, two types of
products can be formed –DCPD and CO3HA.
SEM of the immersed samples in 1.5 SBF solution after 12 days of
soaking are given in Fig.9
Figure 9. SEM of the 50PCL/50BG (a) 20PCL/80BG (b) and 80PLC/20BG
(c) composites after in vitro test in 1.5 SBF for 12 days in static
From the presented SEM images we can see that on the 50PCL/50BG
(Fig. 9, a) and on the 20PCL/80BG (Fig. 9, b) needle-like
hydroxyapatite can be observed[2, 3, 5, 7, 8, 10, 16, 19, 37, 38].
On the other hand, from the depicted in Fig. 9,
International Journal of Materials and Chemistry 2013, 3(5): 91-98
b SEM image, we can also see that the crystallized hydroxyapatite
is nano-needle hydroxyapatite. In the 80PCL/20BG sample we could
see that the surface morphology did not change, because BG was only
20 wt. %. On the base of these results we can conclude that BG was
included in to the PCL matrix.
4. Conclusions The PCL/BG composites have been prepared. BG
synthesized via sol-gel method using TEOS, CaO and H3PO4 as
sources. The nominal composition of BG was 85SiO2-10CaO-5P2O5 (mol.
%). PCL/BG composites were synthesized by mixing of PCL and BG at
20PCL/80BG, 50PCL/50BG and 80PCL/20BG weight ratio. In vitro
bioactivities of the synthesized composites were examined in 1.5
SBF solutions for 3 and 12 days in static conditions. The obtained
samples were characterized by FTIR and SEM. FTIR of the samples
before in vitro test showed that BG was included in to PCL matrix.
After 3 days of soaking in 1.5 SBF solution FTIR observed that the
intensity of the characteristic bands of PCL significantly
decreased. This result can be attributed to the process of partial
dissolution of the organic part of the composites. On the other
hand, some new carbonate bands could be observed. The presence of
these new groups could be related to the carbonate containing
hydroxyapatite, crystallized on the immersed sample. After 12 days
of soaking, FTIR revealed the formation of DCPD and HA on the
surfaces of the immersed samples. The obtained results depict that
the synthesized PCL/BG composites are in v itro b ioactive. SEM of
these samples presented that needle-like HA can be observed. Based
on the presented results we can conclude that the prepared PCL/BG
samples exhib it good in vitro bioactivity.
ACKNOWLEDGEMENTS The authors would like to acknowledge the
PEst-C/CTM/LA0011/2013 for finding this research.
REFERENCES  A. R. Boccaccini, M. Erol, W. J. Stark, D. Mohn, Zh.
F. Mano. Polymer/bioactive glass nanocomposites for biomedical
applications: A review. Composites Science and
 G. Chouzouri, M. Xanthos. In vitro bioactivity and degradation
of polycaprolactone composites containing silicate fillers, Acta
 P. Fabbri, V. Cannillo, A. Sola, A. Dorigato, F. Chiellini,
Highly porous polycaprolactone-45S5 Bioglass® scaffolds for bone
tissue engineering, Composites Science and Technology;70,
 E. Tamjid, R. Bagheri, M. Vossoughi, A. Simchi,Effect of
particle size on the in vitro bioactivity, hydrophilicity and
mechanical properties of bioactive glass-reinforced
polycaprolactone composites, Materials Science and Engineering:
 M. S. Mohammadi, I. Ahmed, B Marelli, Ch. Rudd, M.N. Bureau,
Sh. N. Nazhat, Modulation of polycaprolactone composite properties
through incorporation of mixed phosphate glass formulations, Acta
Biomaterialia;6, 3157-68, 2010
 R L. Prabhakar, S. Brocchini, J. C. Knowles, Effect of glass
composition on the degradation properties and ion release
characteristics of phosphate glass—polycaprolactone composites,
Biomaterials, 26, 2209-18, 2005.
 S. I. Roohani-Estefani, S. Nouri-Khorasani, Z. F. Lu, R.C.
Appleyard, H. Zreiqat, Effects of bioactive glass nanoparticles on
the mechanical and biological behavior of composite coated
scaffolds, Acta Biomaterialia, 7, 1307-18, 2011.
 H.- H. Lee, H.-S. Yu, J.-H. Jang, H.-W. Kim, Bioactivity
improvement of poly(ε-caprolactone) membrane with the addition of
nanofibrous bioactive glass, Acta Biomaterialia, 4, 622-9,
 S.I. Roohani-Esfahani, S. Nouri-Khorasani, Z.F. Lu, M.H. Fathi,
M. Razavi, R.C. Appleyard, et al., Modification of porous calcium
phosphate surfaces with different geometries of bioactive glass
nanoparticles, Materials Science and Engineering: C, 32, 830-9,
 B. Lei, K.-H. Shin, D.-Y. Noh, I.-H. Jo, Y.-H. Koh, H.-E. Kim,
et al., Sol–gel derived nanoscale bioactive glass (NBG) particles
reinforced poly(ε-caprolactone) composites for bone tissue
engineering, Materials Science and Engineering: C, 33:1102-8,
 M. G. Raucci, V. Guarino, L. Ambrosio. Hybrid composite
scaffolds prepared by sol–gel method for bone regeneration,
Composites Science and Technology, 70, 1861-8, 2010
 M. Lebourg, J. Suay Antón, J.L. Gomez Ribelles,
Characterization of calcium phosphate layers grown on
polycaprolactone for tissue engineering purposes, Composites
Science and Technology, 70, 1796-804, 2010
 G. D. Guerra, P. Cerrai, M. Tricoli, A. Krajewski, A.
Ravaglioli, M. Mazzocchi, et al., Composites between hydroxyapatite
and poly(ε-caprolactone) synthesized in open system at room
temperature, J Mater Sci: Mater Med, 17, 69-79, 2006
 M. Lebourg, J. Suay Antón, J. L.G. Ribelles, Hybrid structure
in PCL-HAp scaffold resulting from biomimetic apatite growth, J
Mater Sci: Mater Med., 21, 33-44, 2010.
 S. Joughehdoust, A. Behnamghader, M. Imani, M. Daliri, A. H.
Doulabi, E. Jabbari. A novel foam-like silane modified alumina
scaffold coated with nano-hydroxyapatite –poly (ε-caprolactone
fumarate) composite layer, Ceramics International, 39, 209-18,
 A. Rezaei, M.R. Mohammadi, In vitro study of
hydroxyapatite/polycaprolactone (HA/PCL) nanocomposite synthesized
by an in situ sol–gel process, Materials Science and Engineering:
C;33, 390-6, 2013.
 M. Catauro, M. G. Raucci, F. De Gaetano, A. Marotta, Sol-gel
synthesis, characterization and bioactivity of
98 Lachezar Radev et al.: In vitro Bioactivity of
polycaprolactone /SiO2 hybrid material, J Mater Sci.,38,
 A. Schönbächlera, O. Glaied, J. Huwyler, M. Frenz, U. Pieles,
Indocyanine green loaded biocompatible nanoparticles: Stabilization
of indocyanine green (ICG) using biocompatible
silica-poly(ε-caprolactone) grafted nanocomposites, Journal of
Photochemistry and Photobiology A: Chemistry, 261, 12-9,
 J. Wei, F. Chen, J-W. Shin, H. Hong, Ch. Dai, J. Su, et al.,
Preparation and characterization of bioactive mesoporous
wollastonite – Polycaprolactone composite scaffold, Biomaterials,
30, 1080-8, 2009.
 Y. Lei, B. Rai, K.H. Ho, S.H. Teoh,In vitro degradation of
novel bioactive polycaprolactone—20%tricalcium phosphate composite
scaffolds for bone engineering, Materials Science and Engineering:
C, 27, 293-8, 2007.
 M. Catauro, M. Raucci, G. Ausanio. , Sol–gel processing of
drug delivery zirconia/polycaprolactone hybrid materials, J Mater
Sci: Mater Med., 19, 531-40, 2008.
 Santis RD, M. Catauro, L. D. Silvio, L. Manto, M. G. Raucci,
L. Ambrosio, et al. Effects of polymer amount and processing
conditions on the in vitro behaviour of hybrid titanium
dioxide/polycaprolactone composites, Biomaterials, 28, 2801-9,
 M. Kharaziha, M.H. Fathi, H. Edris. Development of novel
aligned nanofibrous composite membranes for guided bone
regeneration, Journal of the Mechanical Behavior of Biomedical
Materials, 24, 9-20, 2013.
 A. K. Jaiswal, H. Chhabra, S. S. Kadam, K. Londhe, V. P. Soni,
J. R. Bellare. Hardystonite improves biocompatibility and strength
of electrospun polycaprolactone nanofibers over hydroxyapatite: A
comparative study, Materials Science and Engineering: C, 33,
 E. M. Carlisle., Silicon: A Possible Factor in Bone
Calcification, Science, 16, 279-80, 1970
 K. Schwarz, D. Milne, Growth-promoting Effects of Silicon in
Rats, Nature, 239, 333 - 4, 1972.
 J. W. Reid, A. Pietak, M. Sayer, D. Dunfield, T. J. Smith,
Phase formation and evolution in the silicon substituted tricalcium
phosphate/apatite system, Biomaterials, 26, 2887-97,
 N. Y. Mostafa, A. A. Shaltout, L. Radev, H. M. Hassan, In
vitro surface biocompatibility of high-content silicon -
substituted calcium phosphate ceramics., Cent Eur J Chem., 11,
 L. Radev, D. Zheleva, I. Michailova, In Vitro bioactivity of
Polyurethane/85S Bioglass composite scaffolds, Cent Eur J
 M. Tanahashi, T. Yao, T Kokubo, M. Minoda, T. Miyamoto, T.
Nakamura, et al. Apatite Coating on Organic Polymers by a
Biomimetic Proces, J Am Ceram Soc;77, 2805–8, 1994.
 G. Falini, S. Fermani, B. Palazzo, N. Roveri,Helical domain
collagen substrates mineralization in simulated body fluid, J
Biomed Mater Res A., 87, 470-6, 2008.
 Ch. Vaid, S. Murugavel, Alkali oxide containing mesoporous
bioactive glasses: Synthesis, characterization and in vitro
bioactivity, Materials Science and Engineering: C., 33, 959-68,
 D. Arcos, M. Vila, A. López-Noriega, F. Rossignol, E.
Champion, F.J. Oliveira, et al. Mesoporous bioactive glasses:
Mechanical reinforcement by means of a biomimetic process, Acta
Biomaterialia, 7, 2952–9, 2011.
 V. Chiono, G. Vozzi, M. D'Acunto, S. Brinzi, C. Domenici, F.
Vozzi, et al. Characterisation of blends between poly(ε-capr
olactone) and polysaccharides for tissue engineering applications,
Materials Science and Engineering: C., 29, 2174-87, 2009.
 J. Yu, P. Wu, Crystallization process of poly(-caprolactone
)–poly(ethylene oxide)–poly(-caprolactone) investigated by infrared
and two-dimensional infrared correlation spectroscopy, Polymer,
48, 3477-85, 2007.
 M. Catauro, M. G. Raucci, F. de Gaetano, A. Buri, A. Marotta,
L. Ambrosio. Sol-gel synthesis, structure and bioactivity of
Polycaprolactone/CaO • SiO2 hybrid material, Journal of Materials
Science: Materials in Medicine,15, 991-5, 2004.
 F. Yang, J.G.C. Wolke, J.A. Jansen. Biomimetic calcium
phosphate coating on electrospun poly(-caprolactone) scaffolds for
bone tissue engineering, Chemical Engineering Journal,